Corrosion Inhibition of 304 Stainless Steel, Copper and Nickel Metals Using Mesoporous Silicate (MCM- 41) and 2, 5- Distyrylpyrazine Photopolymer
M. B. Zakaria a, M. A. Elmorsi a, and E. M. Ebeid a, b
a Department of Chemistry, Faculty of Science, Tanta University, Tanta, Egypt
b Misr University for Science and Technology (MUST), 6th of October City, Egypt
Mesoporous silicate (MCM-41) and 2, 5-distyrylpyrazine photo- polymer (poly-DSP) were used as corrosion protective coatings for 304 stainless steel, copper and nickel metals. Films on metal surfaces were prepared by dip-coating and vapor deposition (CVD, PVD) methods. Poly-DSP thin films formed by vapor deposition are expected to be incorporated through pores and micro-cracks of SiO2 thin film resulting in extra corrosion protection upon photo polymerization. MCM-41 thin films were characterized by x-ray diffraction (XRD), infrared (IR), BET and electron microscopy (SEM, TEM) techniques. Corrosion protection was studied in 2M HCl aqueous solutions using weight loss and potentiodynamic polarization techniques. The temperature effect on corrosion rates was also studied and the thermodynamic activation parameters of the corrosion reaction were determined. Different corrosion parameters were evaluated including, corrosion current density, corrosion potential, corrosion rate and Tafel constants. The calculated percentage of inhibition efficiencies of the coated electrodes reaches ca 93% in some cases.
A general method to enhance corrosion resistance is to apply protective coatings. The modification of the chemical composition of the coatings can also permit the introduction of other desired chemical and physical properties, such as mechanical strength and hydrophobicity. Various organic coatings have been studied for corrosion protection (1-3). Various oxide coatings obtained by sol-gel processing have been studied extensively for corrosion protection of stainless steel (4-8). In spite of all advantages of sol-gel processing, sol-gel coatings suffer from several drawbacks. Specifically, the high annealing or sintering temperatures (>800 0C) required to achieve a dense microstructure could possibly introduce cracks and/or delamination within the sol-gel coatings (9-12). One viable approach to dense sol-gel derived coatings without post- deposition annealing at elevated temperature is to synthesize organic-inorganic hybrid coatings. Relatively dense hybrid coatings have been developed for applications, including wear resistance (13, 14) and corrosion protection (15-17). Two common methods for preparing coatings on metal surfaces are gaseous, including physical vapor deposition (PVD) and chemical vapor deposition (CVD) methods (18, 19), and liquid phase (20, 21) methods. Most of the ceramic coatings are formed by sol-gel method which requires considerably less equipment and can be amenable to any accessories in a large and complex shape, and is applicable to substrates that cannot withstand high temperatures (22). However, the coatings fabricated by sol-gel process encounter problems of existing pores and cracks
ECS Transactions, 33 (16) 227-243 (2011)10.1149/1.3553173 The Electrochemical Society
227Downloaded 25 Aug 2011 to 18.104.22.168. Redistribution subject to ECS license or copyright; see http://www.ecsdl.org/terms_use.jsp
which may become a detrimental factor to cause delamination and corrosion at the interface of coating and substrates (23). The interest in the sol-gel method for preparation of protective coatings of metallic substrates has nonetheless increased in the last ten years. SiO2 coatings made from tetraethoxysilane (TEOS) have been proposed as oxidation protection of metals since it is one of the best barriers against oxygen diffusion. Although the electrochemical response of these coating is poor due to the presence of residual porosity or micro-cracks that enable the access of the electrolyte to the substrate, the use of alkylalcoxides as precursors effectively improved the performance of these coatings (24). Polymer coatings such as polypyrrole, polyaniline, polyvinyl alcohol, polyethylene glycol, poly(methylmethacrylate) .. etc. have been shown to offer corrosion protection of ferrous and non-ferrous metals (25). Kinlen et al. (26, 27) have shown that polyaniline (PANI) containing organic coating on steel is able to passivate the pinholes and defects in the coating and causes passivation of metal surface through anodization of metal by PANI and formation of an insoluble iron-dopant salt at the metal surface. The inhibition efficiencies of other polymers like polyvinyl alcohol (PVA) and polyethylene glycol (PEG) were evaluated using the weight loss and hydrogen evolution techniques at 30-60C (28). 2, 5- distyrylpyrazine monomer (DSP) is known to undergo four - center type photopolymerization giving highly crystalline 2, 5- distyrylpyrazine photopolymer (poly-DSP) (29). In this article, 2, 5- distyrylpyrazine monomer was incorporated by physical vapor deposition (PVD) in pores and micro-cracks of SiO2 thin films followed by its photo polymerization. This offered extra corrosion protection of stainless steel, copper and nickel metals.
Preparation of mesoporous silicate (MCM 41)
Chemicals. Tetraethyloxysilane (TEOS) (99%) was purchased from Merck. Cetyltrimethyl ammonium bromide (CTAB) (99%) and sodium hydroxide (NaOH) (98%) were purchased from Fluka.
Procedures. 0.46 g NaOH was dissolved into 120 ml H2O with stirring. After the solution becomes clear, 1.4 g CTAB was dissolved completely, and 5.6 ml TEOS was poured into the above solution under vigorous stirring. Stirring was continued for 24 h, and then the mixture was heated at 80 C for 48 h. The mixture was filtered to obtain the silicate solid particles, dried at 100 C for 6 h and the surfactant was removed by calcination at 550 C for 5 h (30). Fabrication of mesoporous silicate (MCM-41) thin films
In the preparation of a uniform nano coating, the pretreatment of the substrate surfaces is important. The metal sheet (2 cm1 cm) was gradually ground using No. 320-1500 emery papers , polished with Al2O3 powder, and then ultrasonically cleaned in acetone , ethanol , and distilled water for 10 min, respectively. After hot air drying, it was coated with nanoparticles. Metal sheets were coated with mesoporous silicate coatings by dip-coating method. In this procedure, the substrate was immersed in the sol solution for 5 minutes then withdrawn at a speed of 0.5-1 mm/s. After drying naturally in the ambience, the specimens were heated in an oven at 150 C for 30 min. Such operation was repeated for four times to increase the coating thickness. Then, the samples were
ECS Transactions, 33 (16) 227-243 (2011)
228Downloaded 25 Aug 2011 to 22.214.171.124. Redistribution subject to ECS license or copyright; see http://www.ecsdl.org/terms_use.jsp
heat-treated at 450 C for 30 min to enable the oxide conversion and removal of solvent and residual organics in the coating. However, during the procedure of densification, crystallization of SiO2 and removal of residual hydroxyl and organic groups, the nano coatings were usually prone to cracking. In order to eliminate the creak defects in the coating and to optimize the coating structure and properties, the nano-SiO2 coated samples were immersed in a boiling water for 10-50 min, and then thermally-treated in the muffle oven again at 450 C for 10 min. Preparation of 2, 5- distyryl pyrazine (DSP) monomer and poly- DSP thin films
2, 5- distyrylpyrazine (DSP) monomer was synthesized according to Probst et.al. (31) using 2, 5- bis ( bromomethyl ) pyrazine as a starting material. The phosphonium salt reacts with benzaldehyde to furnish the desired compound. Photopolymerization of DSP was reported by Masaki Hasegawa et al. in 1967 (32). Since then, a large number of new polymer crystals have been prepared from conjugated diolefinic crystals. All the polymers studied so far, are highly crystalline and three dimensionally oriented with the 1, 3- trans cyclobutane and 1, 4- phenylene groups alternating in the main chain (32). DSP thin films are formed through vapor deposition methods because DSP sublimes at ca. 100 C and is incorporated through pores and micro-cracks of SiO2 thin films. Upon exposure to UV-light (=365 nm), poly-DSP thin films are formed causing extra corrosion protection. Characterization of mesoporosus silicate (MCM-41)
The XRD experiments were performed by using PW 1729 X-ray generator. The XRD patterns were collected using Cu K1 radiation (1.5405 A) at a voltage of 40 kV and current of 30 mA.
The IR measurements were performed by using PERKIN-ELMER 1430 ratio recording infrared spectrophotometer over wave number range from (400 - 4000 cm-1).
N2 adsorption and desorption isotherms were measured at -197 C using a Micromeritics ASAP 2010 apparatus. Prior to experiments, the samples were dehydrated at 350 C until the vacuum pressure was below 5 mHg. The measurement of the surface areas of the samples was achieved by Brunauer-Emmett-Teller (BET) method for relative pressures in the range P/P = 0.0-1.0, and the pore size distributions were determined by Barrett-Joyner-Halenda (BJH) method. The BET method was used for the calculation of surface areas of mesoporous silicate surface by physical adsorption of N2 gas molecules. The Barrett-Joyner-Halenda (BJH) method was used for calculating pore size distributions (33). The method is based on a model of the adsorbent as a collection of cylindrical pores. The theory accounts for capillary condensation in the pores using the classical Kelvin equation, which in turn assumes a hemispherical liquid-vapor meniscus and a well-defined surface tension. The BJH theory also incorporates thinning of the